Download presentation

Presentation is loading. Please wait.

Published byJayden Early Modified over 4 years ago

1
Session 404: Intro to Marine Composites Design-The Basics Dr. Paul H. Miller, PE U. S. Naval Academy

2
Intro to the Intro! Goals: –Traditional methods for marine composites design –A good starting point with some directions –Some lessons learned the hard way (also called case studies) –Some entertainment value!

3
The big however!

4
My assumptions! You have had enough coffee to stay awake! You have some background in composites fabrication –You know what the common fibers and resins are (E-glass, epoxy, etc.) –You know the basic English units of length, force, area, time –You are not an engineer!

5
What is design? (from the dictionary) The purposeful arrangement of parts To create in a highly skilled manner A drawing or sketch

6
What is Marine Composites Design? Intelligent selection and combination of materials (resins, fibers, cores) to create a structure that fulfills a customers requirements Communicating that information!

7
Drawing

8
Or Simple Laminate Table

9
This Seminars Focus Determining the appropriate amount of a given material Some information on selecting materials

10
Design Approaches Numerical methods (number crunching) Experimentation (prototypes) Empirical development (small changes each time) Plagiarism! (Not recommended if you are in college) Also called, benchmarking.

11
Numerical Structural Design Requires: 1.Geometry (what will the part look like, dimensions of length, width, maybe thickness) 2.Loads 3.Material properties, and 4.An analysis method (what theory to use)

12
The Most Fun Part is: Figuring out what it will look like! –In general, smaller parts require less structure, but also require more tooling costs and labor costs –Joints are expensive! –Aim for few parts

13
The Hardest Part is: What are the loads? Brainstorm on all the reasonable ways your customers can abuse your product! Did you think about high heels?

14
Did you think about waves?

15
Easiest Methods Combined methods (loads and analysis). Often called Scantling Rules. Similar to a cookbook. –American Bureau of Shipping (ABS) –Lloyds, DnV, ISO, etc. –Gerrs Elements of Boat Strength –Herreshoffs, etc.

16
Advanced Methods Session 504 topics Loads calculated independently from structural theory CFD, LPT, CLT, FEA, TLA, etc. Potentially more accurate, so potentially lighter and less expensive –break even point?

17
Material Properties To complete a design for strength –Tensile strength –Compressive strength –Shear strength –(Flexural strength) –Fatigue properties For stiffness driven designs –Modulus of Elasticity

18
How to get properties Tables Estimation Tests –Standard –Custom

19
Tables Best Sources –Gibbs & Cox (out of print) –Scott –Greene

20
Scott Tables Example Fig 11 For a 45% resin content, all woven laminate typical of very good hand layup, tensile strength is 36000 psi 36 55 Only for typical mat, cloth and woven roving with polyester (conservative for other resins)

21
Greene Tables Appendix A Example –SCRIMP 7781/epoxy –34% resin content –Tensile strength is 56000 psi! www.marinecomposites.com Free download!

22
Warnings! Tables are usually pretty good if you are using the same resin, cloth and workers as the person who tested them! Many have been burned! –42000 psi compressive strength from carbon/epoxy?! That is half what the table told me! Maintain recommended factors of safety!

23
Property Estimation (from scratch) Micromechanics (Greene has a very good write-up) Example: Stiffness (E) of 55% glass-by-weight glass/polyester cloth laminate Step 1: Fiber volume

24
Estimation (cont) Step 2 Estimate perfect laminate –Rule of Mixtures Step 3 Realize cloth is not all in one direction! Which is about the same as Scott! (We were lucky!)

25
Estimation (cont) Step 4 –Count your blessings if you got a reasonable number and maintain normal factors of safety (2-5)! Step 5 –Try to convince management to pay for a few tests!

26
Thoughts on Materials Boats they are used much see a lot of fatigue (waves, dockings, etc.) Fatigue strengths for a vessel in service for 10 years may be as little as 20% of original values! Brittle resins drive fatigue problems!

27
Simple Composite Fatigue Theory (Dharan) Fatigue endurance limit is 25% of the failure strain of the resin or fiber, whichever is less Failure Strain (elongation) is the percent the material has stretched when it fractures –Poly ~ 1%, VE ~ 3-15%, Epoxy ~3-15% –Glass ~ 4-6%, Carbon ~ 0.4-2%

28
Design for Fatigue (Poly or Epoxy?) Elongation 1%2%3%4%5% E-glass Poly Resin Epoxy Resin Strength Epoxy Laminate Poly Laminate Note: The epoxy laminate is only slightly stronger, but has a much higher fatigue limit! This means the FOS could be lower. Poly Fatigue Epoxy Fatigue

29
Fatigue Rule of Thumb If you want something to last for a long time in operation, choose a resin that has an elongation at failure slightly higher than the fiber you use.

30
Material/Component Testing Test some materials to get peace of mind Prototyping –potato chip Self Experimentation –Navy 44 Test labs (ASTM style tests) Cheapest laminate Try #1!

31
More Tests Most expensive laminate Try #7! 300% more expensive than the first. Final laminate Try #23! Only 40% more expensive than the first, third cheapest Cost of testing was $8K, cost savings for 24 boats was ~$80K

32
Testing Rule of Thumb Current theory can not predict all responses! Choose a test most appropriate to your application. –Boiling test inappropriateness Greene has good summary of common tests

33
American Bureau of Shipping Guide for Building and Classing Offshore Racing Yachts The Elements of Boat Strength by Dave Gerr Two Scantlings Methods

34
Design Example! Scantlings Method What should the hull laminate (solid skin – roving/mat/poly) be for a 30 foot sailboat? Beam is 10, Draft 4, Canoe body depth is 6.5 and weight is 7500 lb. Easiest methods are Gerr and Scott. Stopwatches On!

35
Gerr Method Formula 1-1 –Sn= 30 x 10 x 68 /1000 –Sn= 2 Formula 4-1(and figure) –Lower topside thickness is 0.31 Formula 4-2 –Bottom is 1.15 x Lower topside –Bottom is 0.36 thick Table 4-9 –24-15 Combi is 0.089 so 4 plies!

36
Gerr (cont) Weight is about 0.75 lb/sq ft per ply of 24-15 combi (see Scott Figure 32), so about 3 lb /sq ft for this laminate. Formula 5-5 indicates 6 frames Total time was about 5 minutes. A good way to start!

37
ABS Method Offshore Yacht Guide Section 4.5.4 calls for Combi as standard laminate (Table 4.3) Section 7.3.1 thickness is lower of S=frame spacing C=curvature correction P=load K=panel aspect ratio =strength E=modulus Strength egn Stiffness egn

38
ABS (cont) S=51.4 in (for comparison) C=0.7 P=0.44Fh, F from Table 7.4 = 0.25 h from Table 7.1 = 15 ft x 1.2 for slamming = 18 ft K from Table 7.3 = 0.47 from Table 7.2 = 0.5 x 25000

39
ABS (cont) So, from the first equation, And for the second –K1=0.024 –E = 1.1msi

40
Comparison ABS gave 0.35 and Gerr 0.36! ABS took 30 minutes, Gerr 5 ABS more flexible in material properties (note that if the good laminate in Scott was used, the thickness would be 0.3) ABS open to design geometry variation and has a longer track record. Scott method based on ABS, but more general Greene uses DnV and general equations Note that these were relatively simple examples!

41
For Other Components Use the equations in Scott, Greene and Roarks Formulas for Stress and Strain if you have some engineering background Seriously consider a prototype or mockup!

42
Recommendations for Basic Marine Composites Design Start with Scott for an overview If you are starting from scratch, start with Gerr for the big pieces, use Scott or Greene for preliminary material properties Decide if prototype testing makes sense Get test values of your laminates and use ABS for a second opinion Dont stray too far from the assumptions made by the authors!

43
More Advice! If you have some engineering background, use the more advanced formulas in Greene, Scott and Roarks. Attend Session 504 for more advanced, and potentially rewarding, techniques! Keep a mental list of the 10 dumbest places to save weight on a boat!

44
Contact Information Paul H. Miller Phmiller@usna.edu 410-293-6441 Google Paul H. Miller for my webpages

Similar presentations

OK

Task 2.2 – Identification of most suitable face-sheets and optimization of panel properties Duration: month 1 to month 12 Partners involved: MOTULAB (WP.

Task 2.2 – Identification of most suitable face-sheets and optimization of panel properties Duration: month 1 to month 12 Partners involved: MOTULAB (WP.

© 2018 SlidePlayer.com Inc.

All rights reserved.

To make this website work, we log user data and share it with processors. To use this website, you must agree to our Privacy Policy, including cookie policy.

Ads by Google